One heritage corrosion product less: basic sodium copper carbonate
© The Author(s) 2016
Received: 16 May 2016
Accepted: 10 June 2016
Published: 25 July 2016
The Erratum to this article has been published in Heritage Science 2016 4:35
Basic sodium copper carbonate, Na3[Cu2(CO3)3(OH)]∙4H2O, has been mentioned as heritage corrosion product of copper alloys in two publications. The identification relied on the comparison of the powder diffractograms with ICDD 28-1048. But this erroneous reference card clearly measured chalconatronite, Na2Cu(CO3)2∙3H2O, instead which is indeed the product formed in the synthesis on which the card is based. Therefore, ICDD 28-1048 should be deleted.
KeywordsBasic sodium copper carbonate Chalconatronite Copper corrosion products Sodium tricarbonatohydroxodicuprate(II) tetrahydrate
The aim of the Stuttgart RaCoPhInO programme (‘Rare Corrosion Phenomena of Inorganic Objects’) is to identify hitherto unknown phenomena and compounds occurring during the deterioration of heritage objects. Even after nearly 240 years of scientific studies on heritage objects since the identification of cuprite on a Roman bronze leg in 1779  it is still possible to detect new copper corrosion products. This has been demonstrated recently in our GIMME research (Glass Induced Metal-corrosion on Museum Exhibits) for dicopper formate trihydroxide, Cu2HCOO(OH)3 [2, 3], and sodium copper formate hydroxide oxide hydrate, Cu4Na4O(HCOO)8(OH)2∙4H2O .
But in this case, it is the other way round: we present experimental and theoretical evidence that a rare copper compound identified on metal heritage in the literature is non-existing: basic sodium copper carbonate, Na3[Cu2(CO3)3(OH)]∙4H2O.
The evidence for basic sodium copper carbonate
Nandi and Sengupta [5, 6] reported the synthesis and characterization of the basic sodium copper carbonate Na3[Cu2(CO3)3(OH)]∙4H2O (compound ①, sodium tricarbonatohydroxodicuprate(II) tetrahydrate) in 1972/4. The only other occurrence of ① in the literature identifiable with a Chemical Abstract search (CAS no. 55521-72-7) is our first review of the GIMME phenomenon in 2010 . In the discussion of chalconatronite (Na2Cu(CO3)2∙3H2O, a joint corrosion product of soda glass in contact with copper alloys in clean air free from formaldehyde) it was noted that ① has been mentioned by Barger and White  to occur on a cover glass of a daguerréotype (copper plate with photo-sensitized silver layer). Identified with X-ray Powder Diffraction (XRPD), it was not included in their earlier original research paper on corrosion products . Bellendorf  also identified ① by XRPD together with chalconatronite in five corrosion samples from fourteen to eighteenth cent. burial plates in Franconian chapels in Bamberg and Rothenburg ob der Tauber cast from quaternary copper alloys (Cu/Zn/Sn/Pb). Here the sodium most likely originates from migrating salts in the wall plaster, not from soda glass.
Therefore, we tried to synthesize ① as reference for our GIMME research (e.g., for Raman spectra).
① was prepared by Sengupta and Nandi ‘by adding 50 ml of copper(II) acetate (3.2 g) solution to 250 ml NaHCO3 (10 %). The light blue needle-shaped crystals were filtered, washed and dried’ . Our analyses by XRPD of products obtained that way surprisingly found chalconatronite as only crystalline phase. Rietveld refinement of the pattern proved the presence of amorphous material as well (estimated to 10 to 14 %, depending on washing).
As ① is a basic salt (i.e., it contains a hydroxide anion) in opposite to the ‘neutral’ chalconatronite, one might assume that raising the pH might help to precipitate the basic compound. But by using a sodium hydrogencarbonate/carbonate buffer chalconatronite is definitely synthesized as Sengupta and Nandi report themselves  (see also [11: 353] for a similar synthesis). At even higher pH, by using sodium carbonate (soda) alone, we yielded a totally amorphous product. Gettens and Frondel , the discoverer of the mineral chalconatronite, obtained ‘a pale blue-green precipitate closely similar to chalconatronite in chemical composition… and other properties…simply by grinding in a mortar copper acetate in a saturated solution of sodium carbonate, allowing to stand overnight, filtering, washing and drying.’ Erdös  grew chalconatronite on copper wetted with 10 % soda solution.
By no way, ① could be synthesized. Therefore, the physico-chemical data reported for ① were compared to those for chalconatronite.
X-ray powder diffraction
It is no wonder then that in mixtures were chalconatronite is present also the basic sodium copper carbonate, ICDD 28-1048, can be proposed by peak matching software (as happened for the burial plate samples), and in that way enters analytical reports.
488–494 (b, m) 
490 (m) 
457–566 (b, m) 
562 (m) 
1063 (s) 
1063 (m) 
1350 (d, s)
1380 (d, s)
1600 (s) 
1625 (m) 
1670 (s) 
1670 (m) 
2125–2250 (b, w)
3340–3400 (b, sh) 
3375 (sh) 
3500 (s) 
3550 (s) 
Other physicochemical data reported by Sengupta and Nandi 
The authors found the same effective magnetic moments for ① and for chalconatronite.
The thermogravimetric curves for ① and for chalconatronite differed somewhat, but one cannot assess from the publication if this difference is really beyond normal experimental error or could be caused by the presence of some amorphous material.
Quantitative analytical data for Na+, Cu2+, and CO2 for their precipitate ① led to the supposed formula, they do not fit the stoichiometry of chalconatronite. But we were unable to get a phase pure crystalline compound by their synthesis for ①, 10–14 % amorphous material was present as well. From such a mixture, no meaningful stoichiometric formula can be derived by quantitative analysis of the mixture.
The same holds true for the isothermal weight loss measured for ① and chalconatronite (at slightly different temperatures (150 °C/160 °C).
Our synthetic replication experiments and a closer look at the diffraction data and the IR spectra show that Sengupta and Nandi [5, 6] have synthesized chalconatronite and not the basic sodium copper carbonate ① they postulated. There is no experimental proof of any kind that the latter compound exists at all, neither as lab chemical, nor as corrosion product on heritage objects. Consequently, ICDD 28-1048 should be deleted.
The chalconatronite reference set ICDD 22-1458 of 1969 is still often used in metal heritage corrosion studies (e.g., [16–18]) for identification. To analyse complex mixtures, it should better be replaced by data derived from the crystal structure (e.g., ICDD 01-71-1490 or ) with quantitative values for intensities.
AF performed the synthesis experiments and characterized the precipitates with µ-Raman spectroscopy. RD interpreted the XRD measurements and developed Fig. 1. GE had the idea for this study during a literature survey of rare corrosion products, developed Tables 1 and 2, and wrote the first draft of this communication. All authors read and approved the final manuscript.
We are grateful for the support of this study: C. Stefani performed the XRD measurements. A. Wollmann synthesized a chalconatronite reference sample. P. Bellendorf made copies of his diffractograms available to us. The Glass-Metal Corrosion Research is currently funded by the German Federal Environmental Foundation (DBU, Az. 33255/01).
The authors declare that they have no competing interests.
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The Creative Commons Public Domain Dedication waiver (http://creativecommons.org/publicdomain/zero/1.0/) applies to the data made available in this article, unless otherwise stated.
- Sage M. Observations sur la Mine rouge de Cuivre. Observations sur la Physique, sur l’Histoire Naturelle et sur les Arts. 1779;14:155–57.Google Scholar
- Euler H, Barbier B, Kirfel A, Haseloff S, Eggert G. Crystal structure of trihydroxydicopper formate, Cu2(OH)3(HCOO). Z Kristallogr NCS. 2009;224:609–10.Google Scholar
- Eggert G, Haseloff S, Euler H, Barbier B. When glass and metal corrode together, III: The Formation of Dicoppertrihydroxyformate. J Bridgland editor. ICOM-CC 16th Triennial Conference Lisbon, 19–23 Sept 2011. Lisbon: Critério-Produção. 2011. p. 9.Google Scholar
- Dinnebier RE, Runčevski T, Fischer A, Eggert G. Solid-state structure of a degradation product frequently observed on historic metal objects. Inorg Chem. 2015;54:2638–42.View ArticleGoogle Scholar
- Nandi AK, Sengupta AK. Carbonato Complexes of Copper(II). Proc Chem Symp 1972 Aligarh Muslim University. New Delhi: Dept of Atomic Energy, Gov of India. 1973; Vol. 2:115–120.Google Scholar
- Sengupta AK, Nandi AK. Complex carbonates of copper (II). J Inorg Nucl Chem. 1974;36:2479–84.View ArticleGoogle Scholar
- Eggert G. Corroding glass, corroding metals: survey of joint glass/metal corrosion products on historic objects. Corr Eng Sci Technol. 2010;45:414–9.View ArticleGoogle Scholar
- Barger MS, White WB. The Daguerreotype. Washington (DC): Smithsonian Institution Press; 1991. p. 167.Google Scholar
- Barger MS, Smith DK, White WB. Characterization of corrosion products on old protective glass, especially daguerreotype cover glasses. J Mat Sci. 1989;24:1343–56.View ArticleGoogle Scholar
- Bellendorf P. Metallene Grabplatten aus Franken und Thüringen aus dem 15. bis 18. Jahrhundert—eine interdisziplinäre Studie zum Denkmalbestand und seiner Gefährdung durch Umwelteinflüsse. Ph.D. Dissertation. Bamberg: Otto-Friedrich Universität; 2007. urn:nbn:de:bvb:473-opus-1368.Google Scholar
- Mukhopadyhay U, Bernal I. A totally unexpected synthesis of single crystals of the mineral chalconatronite, Na2(Cu(CO3)2)∙3(H2O), from a solution of a copper coordination compound and atmospheric CO2 at room temperature. J Coord Chem. 2004;57:353–60.View ArticleGoogle Scholar
- Gettens RJ, Frondel C. Chalconatronite: an alteration product on some ancient Egyptian bronzes. Stud Cons. 1955;2:64–75.Google Scholar
- Erdös E. Natriumcarbonatocuprat(II)—trihydrat als Korrosionsprodukt von Kupfer. Corr Sci. 1969;9:435–7.View ArticleGoogle Scholar
- Brotherton D, White AH. Crystal Structures of copper(II) sodium carbonate trihydrate (chalconatronite). J Chem Soc Dalton Trans. 1973;21:2338–40.View ArticleGoogle Scholar
- Taravel B, Berjot M, Fromage F. Étude structurale par spectrométrie infrarouge et Raman du dicarbonatocuprate (II) de sodium. CR Acad Soc Paris Série B. 1974;279:159–61.Google Scholar
- Scott DA. Copper and bronze in art—corrosion, colorants, conservation. Los Angeles: GCI. 2002:424,446.Google Scholar
- Scott DA, Dodd L. Examination, conservation and analysis of a gilded Egyptian bronze osiris. J Cult Her. 2009;3:342.Google Scholar
- Wang Q, Huang H, Shearman F. Bronzes from the sacred animal necropolis at Saqqara, Egypt: a study of the metals and corrosion. Brit Mus Techn Bull. 2009;3:77.Google Scholar
- WWW-MINCRYST (2016). Crystallographic and crystallochemical database for minerals and their structural analogues. http://database.iem.ac.ru/mincryst, accessed 07 Mar 2016. Full Information Card Chalconatronite-835.